Quaternary cerium(iv) containing fluorides exhibiting Ce<sub>3</sub>F<sub>16</sub> sheets and Ce<sub>6</sub>F<sub>30</sub> frameworks.
Ayer, Gyanendra B.; Klepov, Vladislav V.; Pace, Kristen A.; Zur Loye, Hans-Conrad; Dalton transactions (Cambridge, England : 2003) 49 (2020) 5898–5905; doi:10.1039/d0dt00616e

data_7704058
_publ_section_title
;
 Quaternary cerium(iv) containing fluorides exhibiting
 Ce<sub>3</sub>F<sub>16</sub> sheets and Ce<sub>6</sub>F<sub>30</sub>
 frameworks.
;
_journal_issue                   18
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5898
_journal_page_last               5905
_journal_paper_doi               10.1039/d0dt00616e
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'Ce3 Cs2 F16 Mn'
_chemical_formula_weight         1045.12
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_audit_creation_method           SHELXL-2018/1
_audit_update_record
;
2020-02-09 deposited with the CCDC.	2020-04-12 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   7.9014(2)
_cell_length_b                   7.9014(2)
_cell_length_c                   13.0931(4)
_cell_measurement_reflns_used    7557
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      33.09
_cell_measurement_theta_min      2.98
_cell_volume                     707.92(3)
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0354
_diffrn_reflns_av_unetI/netI     0.0096
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            10749
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.490
_diffrn_reflns_theta_min         2.977
_exptl_absorpt_coefficient_mu    15.568
_exptl_absorpt_correction_T_max  0.4954
_exptl_absorpt_correction_T_min  0.3924
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 Reference: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10.
;
_exptl_crystal_colour            'pale brown'
_exptl_crystal_density_diffrn    4.903
_exptl_crystal_description       block
_exptl_crystal_F_000             906
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.747
_refine_diff_density_min         -0.699
_refine_diff_density_rms         0.099
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.090
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     28
_refine_ls_number_reflns         347
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0141
_refine_ls_R_factor_gt           0.0130
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0116P)^2^+2.5491P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0295
_refine_ls_wR_factor_ref         0.0299
_reflns_Friedel_coverage         0.000
_reflns_number_gt                333
_reflns_number_total             347
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0dt00616e2.cif
_cod_data_source_block           Cs2MnCe3F16
_cod_depositor_comments
'Adding full bibliography for 7704051--7704058.cif.'
_cod_original_cell_volume        707.91(4)
_cod_database_code               7704058
_shelx_shelxl_version_number     2018/1
_shelx_res_checksum              40718